Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

- Concrete pavement design, construct... by Rumanshu Katiyar 47032 views
- CONSTRUCTION OF CEMENT CONCRETE ROAD by GLA University 121897 views
- Pavements PPT by Amol Pawar 85837 views
- Witold Zapasnik "Ülevaade betoontee... by Krista Must 237 views
- Continuously reinforced concrete pa... by Chandra Mohan Lodha 349 views
- Long life concrete pavement by Semedar Salim 2536 views

No Downloads

Total views

10,111

On SlideShare

0

From Embeds

0

Number of Embeds

16

Shares

0

Downloads

807

Comments

0

Likes

13

No embeds

No notes for slide

- 1. Concrete Pavement Design Guidance Notes
- 2. Also available from Taylor & Francis Reynolds’s Reinforced Concrete Designer Handbook 11th edition T. Threlfall et al. Hb: ISBN 0–419–25820–5 Pb: ISBN 0–419–25830–2 Reinforced Concrete 3rd ed P. Bhatt et al. Concrete Bridges P. Mondorf Reinforced & Prestressed Concrete 4th ed S. Teng et al. Hb: ISBN 0–415–30795–3 Pb: ISBN 0–415–30796–1 Hb: ISBN 0–415–39362–0 Hb: ISBN 0–415–31627–8 Pb: ISBN 0–415–31626–X Concrete Mix Design, Quality Control and Speciﬁcation 3th ed K. Day Hb: ISBN 0–415–39313–2 Binders for Durable and Sustainable Concrete P.-C. Aïtcin Hb: ISBN 0–415–38588–1 Aggregates in Concrete M. Alexander et al. Hb: ISBN 0–415–25839–1 Information and ordering details For price availability and ordering visit our website www.tandf.co.uk Alternatively our books are available from all good bookshops.
- 3. Concrete Pavement Design Guidance Notes Geoffrey Griffiths and Nick Thom
- 4. First published 2007 by Taylor & Francis 2 Park Square, Milton Park, Abingdon, Oxon OX14 4RN Simultaneously published in the USA and Canada by Taylor & Francis 270 Madison Ave, New York, NY 10016 Taylor & Francis is an imprint of the Taylor & Francis Group, an informa business This edition published in the Taylor & Francis e-Library, 2007. “To purchase your own copy of this or any of Taylor & Francis or Routledge’s collection of thousands of eBooks please go to www.eBookstore.tandf.co.uk.” © 2007 Geoffrey Grifﬁths & Nick Thom All rights reserved. No part of this book may be reprinted or reproduced or utilised in any form or by any electronic, mechanical, or other means, now known or hereafter invented, including photocopying and recording, or in any information storage or retrieval system, without permission in writing from the publishers. The publisher makes no representation, express or implied, with regard to the accuracy of the information contained in this book and cannot accept any legal responsibility or liability for any efforts or omissions that may be made. British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library Library of Congress Cataloging in Publication Data Grifﬁths, Geoffrey. Concrete pavement design guidance notes / Geoffrey Grifﬁths and Nicholas Thom. p. cm. Includes bibliographical references and index. 1. Pavements, Concrete. I. Thom, Nicholas. II. Title. TE278.G75 2007 625.8 4–dc22 ISBN 0–203–96206–0 Master e-book ISBN ISBN10: 0–415–25451–5 (hbk) ISBN10: 0–203–96206–0 (ebk) ISBN13: 978–0–415–25451–9 (hbk) ISBN13: 978–0–203–96206–0 (ebk) 2006020039
- 5. This book is dedicated to the engineer who thought he knew how to calculate the stresses or strains in a working concrete pavement.
- 6. Contents List of ﬁgures List of tables List of equations Acknowledgements Notations 1 Introduction 1.1 1.2 1.3 1.4 1.5 1.6 1.7 2 2.5 2.6 2.7 1 Background 1 Standard design methods 2 Calculating stress 2 Economic viability of concrete pavement systems 2 A note on concrete 3 Units 4 Reference 4 Surface slab systems 2.1 2.2 2.3 2.4 xi xiii xv xviii xix Description of systems 5 Unreinforced concrete (URC) pavements 6 Jointed reinforced concrete (JRC) pavements 9 Continuously reinforced concrete (CRC) pavements 13 Variant slab systems 17 Summary 18 References 18 5
- 7. viii 3 Contents Concrete bases and sub-bases 3.1 3.2 3.3 3.4 3.5 3.6 4 5 Introduction 21 Roller compacted concrete (RCC) systems 23 Flexible composite systems 24 CBM sub-base systems 25 Summary 27 References 27 Testing and speciﬁcation 4.1 4.2 4.3 4.4 4.5 4.6 4.7 21 29 Introduction 29 Standard strength test methods 29 In situ pavement compaction and strength 38 Concrete fatigue 40 Durability 43 Speciﬁcation 46 References 53 Concrete slab analysis methods 55 5.1 5.2 5.3 5.4 5.5 5.6 5.7 Introduction 55 Westergaard analysis 55 Slab bending expressions 56 Limit state bearing capacity calculation 61 Westergaard and Meyerhof techniques compared 68 Treatment of multiple loads 69 Factors reducing the validity of semi-empirical design methods 70 5.8 Useful relationships for composite slabs 73 5.9 Implications for pavement design 75 5.10 References 76 6 Design inputs and assumptions 6.1 6.2 6.3 6.4 6.5 6.6 6.7 Introduction 77 Trafﬁc characterisation and design life 77 Aircraft loading 82 Pavement foundations 82 Probability and risk 90 Conclusions 93 References 94 77
- 8. Contents 7 Concrete pavement design methods ix 97 7.1 7.2 Introduction 97 AASHTO guide for design of pavement structures 1992 97 7.3 AASHTO interim guide 1998 design method 103 7.4 TRL research report 87 103 7.5 Airﬁeld pavement designs 109 7.6 Port pavements 112 7.7 Other Westergaard-derived methods and TR550 113 7.8 Other Meyerhof-derived methods and TR34 114 7.9 Discussion and recommendations 115 7.10 References 117 8 Composite pavement design 8.1 8.2 8.3 8.4 8.5 8.6 8.7 8.8 8.9 9 Introduction 119 The AASHTO design method 120 UK standard designs 123 UK Technical Paper PE/TP/169/92 124 The South African method 128 The French method 130 Reﬂective cracking 131 Discussion 131 References 131 Joints 9.1 9.2 9.3 9.4 9.5 9.6 9.7 9.8 9.9 9.10 9.11 119 133 Introduction 133 Joint efﬁciency 133 Load transfer devices 134 Joint sealing 136 Joint types 138 URC joint detailing 141 JRC joint detailing 143 CRC joint detailing 145 Strong CBM jointing 145 Conclusions 146 References 146
- 9. x Contents 10 Detailing 10.1 10.2 10.3 10.4 10.5 10.6 10.7 10.8 10.9 Index 149 Introduction 149 Minimum layer thickness 149 Surface ﬁnish 150 Slip membranes 154 Highway carriageway rollovers 157 Transitions between different types of construction 157 Slip road connections into a main carriageway 158 CRCP anchorages 158 References 162 165
- 10. Figures 2.1 2.2 2.3 2.4 2.5 3.1 3.2 4.1 4.2 4.3 4.4 4.5 4.6 4.7 4.8 4.9 4.10 5.1 5.2 5.3 5.4 5.5 5.6 5.7 6.1 6.2 6.3 7.1 7.2 7.3 A typical URC pavement Typical structural failure in URC pavements A typical JRC pavement A typical CRC construction Typical shapes used for reinforcing ﬁbres Approximately equivalent composite systems Deterioration of a ﬂexible composite pavement Strength testing of concrete samples Bending stress/strain in a mass concrete beam Summary of compressive cube to ﬂexural strength data Fatigue data and design models UK CBM sub-base grading curves UK CBM base grading curves Seven-day cube strength data against time Twenty-eight-day core strength data against time Estimated ﬂexural strength at 28 days Relationship between cube and core density and strength in a pavement project Westergaard Internal, Edge and Corner loading The deﬂected shape of an internally loaded slab The formation of plastic hinges Limiting moment in a mass concrete slab Limiting moment in a centrally reinforced concrete slab The inﬂuence of adjoining slabs on pavement deﬂection Summary of environmental effects Standard UK truck axle loads UK and US methods linking k762 and CBR RR87 calibration and reliability adjustments for URC URC systems designed over a granular sub-base JRC systems over a granular sub-base JRC systems over a CBM sub-base 6 9 10 14 17 22 25 30 34 37 42 48 48 50 50 51 51 56 58 62 66 66 71 72 81 86 92 105 107 107
- 11. xii 7.4 7.5 7.6 9.1 9.2 9.3 9.4 9.5 9.6 9.7 9.8 9.9 10.1 10.2 10.3 10.4 10.5 10.6 10.7 10.8 Figures CRC systems over a granular sub-base CRC systems over a CBM sub-base FAA designs for Boeing 747-400 loading Joint efﬁciency Possible joint construction problems Joint sealant details Transverse joint types Longitudinal joint types Expansion joint Isolation joint URC joint layout A circular bend jointing layout Concrete pavement surface ﬁnishes The impact of slip membranes on crack-induced joints Effect of omitting movement joint between ﬂexible and rigid construction Transition from rigid to ﬂexible construction Connection of slip roads into a main carriageway UK standard I-beam termination system UK reinforced concrete ground beam details Dutch reinforced concrete ground beam system 109 109 111 134 135 137 139 140 141 142 143 144 155 156 158 158 159 161 161 162
- 12. Tables 2.1 2.2 2.3 2.4 4.1 4.2 4.3 4.4 4.5 5.1 5.2 6.1 6.2 6.3 6.4 6.5 6.6 6.7 6.8 7.1 7.2 7.3 7.4 7.5 7.6 8.1 9.1 9.2 Maximum UK recommended joint spacing URC pavements German standard URC pavement design options Maximum joint spacing for JRC pavements Typical UK pavement designs; 40 MPa strength Summary of coefﬁcients of thermal expansion The effect of entrained air on concrete strength Summary of UK CBM strength assumptions Summary of materials testing results from a UK airﬁeld project Summary of standard test methods Westergaard and Meyerhof calculated stresses compared Equivalent concrete thickness from Asphalt surfacing US and UK axle loads and damage factors Damage exponents used in South Africa Factors used in French method Summary of damage factors using different methods AASHTO sample effective modulus calculation Summary of RR87 foundation stiffness computations Standard support platform cases Standard support platform stiffness calculations Summary of AASHTO design example Summary of AASHTO 1998 interim guidance designs Summary of RR87 calculated thicknesses Summary of RR87 JRC designs with A393 reinforcement Summary of RR87 CRC designs TR550 design examples AASHTO derived composite pavement thicknesses Joint sealant dimensions, UK Highways Agency Summary of joint spacing requirements 7 9 10 18 43 45 47 50 52 69 75 79 80 80 82 88 89 89 90 100 103 105 106 108 114 122 137 142
- 13. xiv Tables 9.3 9.4 10.1 10.2 10.3 JRC joint spacing CRC system joint spacing Summary of surface characteristics The inﬂuence of surface ﬁnish on ride quality Seasonal movements in unrestrained CRCP 144 145 151 152 160
- 14. Equations 4.1 4.2 4.3 Tensile splitting strength Tensile splitting strength to tensile axial strength Tensile splitting strength to cylinder strength after Oluokun et al. 4.4 Young’s Modulus derived from ITSM testing 4.5 Tensile ﬂexural strength 4.6 Flexural strength to axial strength relationship 4.7 General cube strength to ﬂexural strength relationship 4.8 Compressive cube strength to ﬂexural strength after Croney and Croney 4.9 Tensile splitting strength to compressive splitting strength after De Larrard 4.10 Relationship between strength and time from CEM Code 90 4.11 Tensile splitting strength to tensile axial strength 4.12 Young’s Modulus values 4.13 The PCA fatigue design relationships 4.14 The PCA 50% probability relationship 5.1 Radius of relative stiffness; liquid foundation 5.2 Radius of relative stiffness; elastic solid foundation 5.3 Westergaard Internal loading and deﬂection expressions 5.4 Loseberg Edge stress and deﬂection expressions 5.5 Kelly’s empirical Edge stress expression 5.6 Westergaard Corner stress and deﬂection expressions 5.7 Pickett’s empirical Corner stress expression 5.8 Meyerhof Internal moment expression 5.9 Meyerhof Edge moment expression 5.10 Meyerhof Corner moment expression 5.11 Limiting moment of resistance Mo 5.12 Limiting moment of resistance for mass concrete slabs, Internal and Edge load cases 32 32 33 33 34 35 36 36 36 39 40 40 43 43 56 57 57 59 59 60 61 62 63 63 64 64
- 15. xvi Equations 5.13 5.14 5.15 5.16 5.17 5.18 5.19 5.20 5.21 5.22 5.23 5.24 5.25 5.26 5.27 6.1 6.2 6.3 6.4 6.5 6.6 6.7 6.8 6.9 6.10 7.1 7.2 7.3 7.4 8.1 8.2 8.3 8.4 8.5 8.6 8.7 Limiting moment of resistance for reinforced concrete slabs, Internal and Edge load cases Limiting moment of resistance for reinforced concrete slabs, Corner load case Limiting moment of mass concrete slabs Net moment of longitudinal and transverse reinforcement Limiting moment reinforcement, centrally reinforced slab Limiting moment concrete compression, centrally reinforced slab Radius of curvature of the slab I neutral axis centrally reinforced slab (describing the section in terms of concrete) Meyerhof internal moment treatment for multiple wheels Bradbury empirical temperature relationship Radius of curvature unbonded two layer slab Unbonded two layer slab moment of resistance Equivalent slab thickness expression Distance from base to neutral axis Two layer, bonded system Power law and trafﬁc damage DCP to CBR relationship Kleyn and Van Heerden (60◦ cone) Adjustment factor to plate size to obtain k762 Surface stiffness modulus MR Surface modulus to CBR relationship k762 to CBR k762 to CBR Relative damage factor Uf Resilient modulus to relative damage factor Normal distribution reliability adjustment to a design AASHTO basic equation for URC pavement design AASHTO reinforcement detailing equation RR87 design equation for URC pavement RR87 design equation for JRC pavement AASHTO basic equation for ﬂexible pavement design AASHTO equation to estimate layer thickness Design stress in CBM materials Thermal warping stress calculation after Thomlinson A1 adjustment after Thomlinson K1 thermal warping stress adjustment after Bradbury South African CBM fatigue life acceptance criteria for Category A roads 64 65 65 67 67 67 68 68 69 72 73 73 74 74 74 78 83 84 85 85 85 86 87 87 92 98 101 104 106 120 120 124 125 126 126 129
- 16. Equations South African CBM crushing initiation life acceptance criteria for Category A roads 8.9 South African CBM advanced crushing life acceptance criteria for Category A roads 8.10 French maximum permitted tensile stress requirement 9.1 Joint efﬁciency 10.1 To predict unrestrained movement in CRCP xvii 8.8 129 129 130 134 160
- 17. Acknowledgements We owe an immense debt to the staff at the University of Nottingham for their initial guidance in introducing us to the design of concrete pavements through their MSc course in Highway Engineering. We would like to thank the following staff for their interesting lectures around the subject of pavement engineering: • • • Professor E. Barenberg for his visiting week of lectures in 1994; Andrew Dawson for his opinions on the design of pavements; Dr Kim Elliot for the quality of his notes on concrete design. The book also owes a substantial debt to Britpave, the UK concrete pavement association, David Jones, the Director and the many industrial members of the group. In particular we would like to thank Graham Woodman of WSP, Bob Lane from BAA and Jonathan Green. Britpave has provided a stimulating forum for the debate of issues associated with concrete pavements. I must also thank my fellow colleagues at Ove Arup & Partners who have, over the years, offered me the opportunity to work on many major prestigious civil engineering projects around the world. We would like to thank the following organisations for permission to reproduce certain material in this text: • • • TRL Figure 6.3, Table 6.6, Equations 6.5, 7.3, 7.4 American Concrete Pavement Association Figure 9.7 HMSO Figures 10.5, 10.6, 10.7
- 18. Notations Chapter 4 ft,sp = tensile splitting stress F = applied force l = cylinder or cube length d = cylinder diameter or cube length ft,axl = tensile axial stress fc,cyl = compressive cylinder strength fc,cube = compressive cube strength ft,ﬂ = tensile, ﬂexural strength F = applied load L = distance between supporting rollers d = beam depth b = beam width ft,axl = mean tensile axial strength hb = slab thickness β = factor to adjust 28-day strength S = cement factor, 0.25 for normal and rapid hardening cement, 0.38 for slow hardening cement T = number of days since construction Eci = Initial Tangent Young’s Modulus for dynamically loaded uncracked material C = correction factor, speciﬁc to a material Ec = static uncracked Young’s Modulus (Secant Modulus) Elong-term = long-term static uncracked Young’s Modulus ft,ﬂ = ﬂexural tensile strength from the standard beam test σt,ﬂ = tensile stress calculated under a design load R = ratio maximum to minimum stress within the loading cycle t = duration of loading pulse N = the number of load repetitions to failure
- 19. xx Notations Chapter 5 = radius of relative stiffness (m) k = modulus of subgrade reaction, = stress/deﬂection (Pa/m; normally quoted as MPa/m) E = Young’s Modulus of pavement slab (Pa; normally quoted as GPa) h = Thickness of the pavement slab (m) ν = Poisson’s Ratio of the pavement slab Es = Young’s Modulus of the subgrade, considered as inﬁnitely thick (Pa; normally quoted as MPa) νs = Poisson’s Ratio of the subgrade P = applied load (N) a = radius of contact area for the point load (m) a1 = distance from the load centre to the corner = 20.5 a Mo = limiting moment of resistance of the slab per unit length Mn = negative moment of resistance Mp = positive moment of resistance Mc = limiting moment of resistance for mass concrete slab per unit length Ms = limiting moment of resistance for reinforced concrete slab per unit length ft = concrete tensile stress at failure h = thickness of concrete slab Ms = net resultant moment as = net resultant area of reinforcement Mt = transverse moment at = area of transverse reinforcement Ml = longitudinal moment al = area of longitudinal reinforcement MS = limiting moment of resistance for centrally reinforced concrete slab per unit length fs = steel tensile stress at failure as = net resultant area of reinforcement h = thickness of concrete Mcc = limiting moment concrete compression per unit length d = effective depth of section X = depth as described in Figure 5.5 and Equation 5.18 m = separation of dual wheels t = separation of tandem wheels E = Young’s Modulus of concrete (MPa) α = coefﬁcient of thermal expansion (per ◦ C) T = temperature difference, top to bottom of slab (◦ C) ν = Poisson’s Ratio Lx = distance between joints in x direction Ly = distance between joints in y direction
- 20. Notations xxi = radius of relative stiffness h1 , h2 = thicknesses of slabs 1 and 2 E1 , E2 = Young’s Moduli of slabs 1 and 2 M1 , M2 = bending moments experienced by slabs 1 and 2, per m length σ1t , σ2t = maximum tensile stresses in slabs 1 and 2 under applied moment M0 M0 = applied moment per m length Chapter 6 F = ‘damage factor’ applicable to axle load P (also known as ‘equivalence factor’ or ‘wear factor’) P = axle load in kN Ps = standard axle load in kN n = relative damage exponent, commonly taken as 4 hdesign = design pavement thickness hmean = mean pavement thickness based around a calculation Z = normal distribution adjustment S = standard deviation based on the calculation and construction variability Chapter 7 W18 = trafﬁc loading in standard 18 kip (80 kN) axles D = pavement thickness in inches Ec = Young’s Modulus of concrete in psi k = modulus of subgrade reaction in pci Sc = the mean 28-day modulus of rupture – that is ﬂexural strength So = the standard deviation of the data used to construct the pavement ZR = values (for a statistically normal distribution) J = values: joint factor CD = drainage coefﬁcients PSI = change in pavement serviceability index during pavement life Po = initial serviceability condition Pt = terminal serviceability condition Ps = percentage steel reinforcement L = slab length, the distance between free Edges (feet or m) F = friction factor at the base of the slab, 1.8 for lime, cement or bitumen stabilised material, 1.5 for unbound gravel or crushed stone and 0.9 for natural subgrade fs = ultimate fracture stress of reinforcement used in the slab (psi or MPa) ft = indirect tensile strength, mean 28-day value used in design Sc = ﬂexural strength (i.e. modulus of rupture), mean 28-day value RT = aggregate factor taken as: gravel = 5/8, crushed rock 2/3
- 21. xxii Notations Ln = Naperian (or natural) logarithm L = pavement life in msa H = pavement thickness in mm S = 28-day mean cube compressive strength in MPa M = equivalent foundation modulus beneath the concrete slab in MPa (see Chapter 6) F = percentage of failed bays R = is the amount of reinforcement in mm2 /m measured as cross-sectional area of steel per metre width of slab Chapter 8 W18 = trafﬁc loading in standard axles ZR = adjustment to give different levels of conﬁdence in design MR = subgrade surface modulus in psi So = the standard deviation of the data used to construct the pavement, taken as 0.35 PSI = serviceability loss (see Chapter 7, Section 7.2.1) Sn = pavement ‘structural number’, a measure of the intended pavement strength ft,ﬂ = the 28-day mean ﬂexural strength σtr = the trafﬁc-induced stress from a 40 kN wheel load σtherm = the thermally induced warping stress at the underside of the CBM layer σtherm = thermally induced stress E = CBM stiffness modulus, taken as 29 GPa for CBM3G α = coefﬁcient of CBM expansion, taken as 12 × 10−6◦ C−1 for all standard calculations θ = amplitude of diurnal temperature variation ν = Poisson’s Ratio, taken as 0.15 ah = thickness coefﬁcient, related to a standard set of factors in Nunn’s work H = composite slab thickness (mm), taken as CBM thickness d = diffusivity factor taken as (0.9)0.5 = 0.94 T = the periodic time cycle Neff = estimated pavement design life for Phase 1 ζ = maximum calculated strain in the pavement ζb = default material strain value Nci = estimated design life for Phase 2 σv = maximum calculated stress at the top of the CBM layer UCS = default unconﬁned compressive strength for the test material σt,ad = the adjusted strength of the CBM layer σt, (NE) = bending failure stress (ﬂexural strength) on a sample at 360 days
- 22. Notations xxiii kr = adjustment for reliability, the example in the text [6] uses a value of 0.744 kd = adjustment to reﬂect joints and cracks in the CBM layer, taken as 1.25 kc = calibration adjustment to the calculation, taken as 1.4 or 1.5 for different CBM materials ks = adjustment for the reduction in bearing capacity due to laying material over weak subgrade Chapter 10 Ses is the season of placement; 1.33 for summer, 1.0 winter h = concrete slab thickness (m) α = ‘thermal coefﬁcient’, expressed in strain per ◦ C f = sub-base frictional factor; 0.037 plastic sheeting, 0.0086 asphalt base, 0.0031 cement treated base
- 23. Chapter 1 Introduction 1.1 Background Concrete pavements are a frequently misunderstood form of construction. Many practising engineers are unaware of the basic design issues which should really be understood before undertaking the construction of any pavement in concrete. Most engineers receive extensive training in the design of reinforced concrete structures but very little formal training is given in the design of concrete pavements. Yet concrete pavements are designed quite differently from reinforced concrete structures. This document presents an explanation of the various design methods, materials testing methods, speciﬁcations and details that are associated with construction of cement bound (i.e. concrete) pavements. The design of concrete pavements has to be treated in a different manner from that of bituminous or granular pavement systems. This book is written partly out of despair; UK pavement design lacks a clear accepted text deﬁning the terminology and methods employed within the concrete pavement industry and much confusion currently exists in describing pavement materials, strengths and loadings. Of course, a single book can never be perfect, but this one is intended to be a working script that will assist an engineer and, where appropriate, point towards other references. The chief aim of this book is to summarise the main design methods in use in the UK and USA, although reference will also be made to methods elsewhere where they are seen as particularly appropriate. The book is clearly unable to draw together every piece of current information or opinion in the ﬁeld; however, every effort has been made to be as accurate as possible within the conﬁnes of the need to produce a concise but informative script on the subject. The book is not a code of practice or design method; engineers must use the original design standards precisely to produce pavement designs.
- 24. 2 Introduction 1.2 Standard design methods A successful design method must include each of the following key elements: • • • • • a standard description of loading; a technique for describing the subgrade support and the required foundation design; a method to determine pavement strength (commonly undertaken as a Westergaard-derived stress calculation); calibration; anchoring the method against data from pavement trials; a speciﬁcation, to control construction materials and techniques. A number of standard methods may be used to produce successful pavement designs. But it is important that practising engineers understand that the different design techniques cannot be mixed and matched. None of the design methods is a precise model of the real world; each method calculates pavement thickness in a different way. If sections taken from different methods are combined inappropriately, the basis of the design is lost. Thus, an AASHTO design must be produced exactly in accordance with the AASHTO method and constructed in accordance with the AASHTO speciﬁcation. Mixing and matching design methods reduces the accuracy of a design. 1.3 Calculating stress Another important reason for writing this book is that many young designers appear to think that substantial beneﬁts may be obtained if only one can calculate the stress within the pavement. Analysing concrete pavements appears to be rather like the mediaeval alchemists’ quest to turn base metal into gold; the quest can never be achieved. Experienced engineers realise that their calculations are imperfect and cannot ever exactly match real site conditions. Engineers should understand that their calculations are no more than estimates and artistic descriptions of pavement failure. All pavement engineering is a subtle blend of art and science, and concrete pavement engineering is no exception. 1.4 Economic viability of concrete pavement systems Yet another excellent reason for writing this book is that concrete is commonly the cheapest form of construction for large heavily trafﬁcked pavements. The economics of concrete pavement construction becomes even more attractive if large quantities of sand and gravel are present on site. Large areas of central Europe have vast reserves of sand and gravel but no hard
- 25. Introduction 3 stone aggregates. Concrete pavements are particularly attractive solutions to the construction of large infrastructure projects in these areas. It should also be noted that concrete pavements are often particularly appropriate in hot climates or situations where very low subgrade strengths may occur. However, concrete pavements are currently suffering from a poor public relations image. Many members of the public have driven over poorly constructed jointed concrete motorways and perceive them as both noisy and bumpy when compared with bituminous surfaces. The bitumen industry has also supported a number of design guides that have improved the competitive perception of bituminous roads. This design guide is intended to assist practising engineers in ensuring that when concrete is considered it is used correctly and, if economically attractive, also constructed successfully. 1.5 A note on concrete This is most certainly not a book about concrete. It is a book about the use of concrete in a particular application, namely pavements, and that means that it is only necessary to understand concrete as a material having certain relevant properties. Thus, the type and size of aggregate used, the cement and water contents, are only important here in terms of the way they affect the engineering properties of the ﬁnished product. There are numerous excellent texts, notably Neville [1], which deal in detail with concrete as a material. In brief, the key properties of interest here are: • • • • Strength – the stress required to cause fracture; Fatigue characteristics – the tendency to fail at a stress lower than the fracture strength if enough load applications (e.g. truck wheels) are applied; Stiffness – the ratio of applied stress to resulting strain; Expansion coefﬁcient – the relative increase in dimension as temperature increases. Of course, it is necessary to have a certain appreciation of how the material is produced (usually in a batching plant) and how it is incorporated into a pavement (either wet formed or laid dry and roller compacted). Similarly, the fact that all concretes take a certain time to gain strength has consequences which impact on design and speciﬁcation, as does the fact that they inevitably shrink measurably during the strength gain process. Concrete materials will also shrink and warp as they cure or age. However, here it will simply be assumed that the appropriate techniques are employed during this ‘curing’ process to make sure that shrinkage cracks are avoided and that loading is not applied prematurely. The actual processes and the different curing rates induced by different types of cement and at different temperatures are not issues dealt with here.
- 26. 4 Introduction 1.6 Units This book is written principally using the SI system of units. The majority of the calculations presented are performed using metres, newtons, pascals, etc.; imperial units (inches, pounds, psi, etc.) are only used when alternative metric units would clearly cause confusion, which in practice means when illustrating certain American computational approaches. 1.7 Reference 1. Neville, A.M., Properties of Concrete, 4th edn, Longman Scientiﬁc and Technical, New York, 1995.
- 27. Chapter 2 Surface slab systems 2.1 Description of systems Surface slab systems, otherwise known as ‘rigid’ pavements, are the most easily recognised form of cement bound pavement construction. Three alternative and interchangeable forms are commonly found in civil engineering projects: • • • mass concrete slabs or unreinforced concrete (URC); jointed reinforced concrete (JRC); continuously reinforced concrete (CRC). Concrete surface slab systems have speciﬁc advantages when compared with bituminous pavements; a concrete pavement consists of a system of stiff plates connected together to form a continuous, hinged slab system. The speciﬁc advantage of a concrete pavement is that the relatively rigid plates apply load over a wide area. Concrete surface slab systems are useful when: • • • low subgrade strengths are anticipated; exceptional heavy point loads will be encountered; low ﬂashpoint petrochemical spillage may be expected. The essential features of a concrete slab system are: • • • • The pavement will include a system of joints which may be natural cracks, as in CRC, or formed joints as in URC or JRC. The tensile capacity of the concrete represents a substantial component of the pavement’s strength. The surface ﬁnish must be designed to be resistant to abrasion, frost and also to provide a serviceable skid resistant surface. The pavement edge and kerb detail can contribute to the strength of the pavement. An untrafﬁcked shoulder acts as a rigid beam stiffener increasing the pavement strength.
- 28. 6 Surface slab systems Each of the three distinct forms of concrete pavement are described and discussed in this chapter. 2.2 Unreinforced concrete (URC) pavements Unreinforced mass concrete pavements consist of a system of (usually) rectangular panels connected together by transverse and longitudinal joints. One of the most important elements of URC pavement design is to ensure that the joints are detailed and, most importantly, spaced correctly. The pavement joints must be arranged to produce a patchwork of roughly square panels with longitudinal joints running in one direction and transverse joints running at 90◦ – except where geometric constraints absolutely demand that a different angle is used locally. Figure 2.1 shows a typical pavement layout. Joint spacing is controlled by standard practice and is a function of pavement thickness; thicker pavements allow greater joint spacing. Table 2.1 details accepted UK practice for joint spacing. It is noted that the recommended maximum ratio of longitudinal joint spacing to transverse joint spacing is 1.25. Pavement joints may be constructed as plain, dowelled or tied (see Chapter 9); current practice is to construct most highway pavements b e a d i h c Key a b c d e f g h i g slab width, between longitudinal joints slab length, between transverse joints support platform trowelled border pavement surface finish tie bar (longitudinal joint) dowel bar (transverse joint) slab thickness slip membrane Figure 2.1 A typical URC pavement. f
- 29. Surface slab systems 7 Table 2.1 Maximum UK recommended joint spacing URC pavements [1] Slab thickness (mm) Transverse joint spacing Longitudinal joint spacing Any aggregate (m) Limestone (m) Any aggregate (m) Limestone (m) 150 200 250 300 3.7 4.6 5.0 6.0 4.5 5.5 6.0 7.0 3.7 4.6 5.0 6.0 4.5 5.5 6.0 7.0 with dowels and tie bars. Omitting the steel dowels or tie bars reduces the efﬁciency of the joint and demands an increase in pavement thickness. The pavement will usually include a slip membrane (see Chapter 10); a bituminous de-bonding membrane is the most efﬁcient form of construction for crack-induced joints, plastic sheet membranes should only be used with dowelled or tied joint details. The maximum recommended highway trafﬁc for untied joints is suggested as 1.5 million standard 80 kN axles (msa – see Chapter 6) or about 1.4 million HGV load applications, although airports and industrial pavements with very thick concrete slabs often make use of plain joints. Joint sealing is essential for all heavily trafﬁcked pavements. The main function of the joint seal is to: • • Prevent debris from falling down the gap between adjacent slabs. A clogged joint is unable to expand in response to raised temperature. If the pavement becomes restrained, high temperatures can result in ‘blow ups’ and compression failure. Prevent moisture ingress, which can lead to softening of pavement foundation materials and, in extreme cases, ‘pumping’ of sub-base ﬁnes to the surface. URC applications Examples of successful forms of mass concrete pavement construction are: Airﬁeld pavements Large, strong, 350–450 mm thick, usually slip-formed areas of concrete are constructed with sawn, crack-induced joints. US practice uses dowels and tie bars; UK pavements generally have plain joints. The pavements are built over a slip-formed lean-mix concrete support platform and a bituminous sprayed
- 30. 8 Surface slab systems de-bonding membrane. The lean-mix acts as support to the crack-induced joints, preventing ‘faulting’. A typical UK pavement designed for Boeing 737 loading in accordance with the widely used PSA Design Guide [2] will consist of: • • • • • • concrete surface brush ﬁnished (see Chapter 10); 320 mm URC, 40 MPa 28-day characteristic compressive cube strength, air entrained concrete; plain, crack-induced joints; a bituminous, sprayed de-bonding membrane; 150 mm lean-mix concrete, 20 MPa 28-day characteristic compressive cube strength; 5% CBR subgrade. Bombay city streets The city currently uses mass concrete as a standard pavement option. The mass concrete pavement is preferred to an alternative bituminous option as the pavement is considered to be more durable in the hot, humid climate. The Paciﬁc motorway, Queensland, Australia A substantial section of this recently constructed motorway is built as plain-jointed URC pavement. The highway consists of a section of dual 3-lane and the remainder is dual 2-lane highway. Concrete was used as it was reported [3] to be the most economic solution. The typical pavement construction is as follows: • • • • • 250 mm URC, 40 MPa 28-day characteristic compressive cube strength; 125 mm lean-mix concrete; 150 mm unbound granular material; 300 mm selected capping, minimum soaked or in situ CBR 7%; 3% CBR subgrade. German Autobahn construction Three different variations on a URC pavement are currently included in the German Federal Standard. Standard URC pavements are constructed with joints at 5 m centres. Each lane is divided into separate slabs. The standard designs are described in Table 2.2. The pavement surface is ﬁnished in: • • either a burlap ﬁnish in a longitudinal direction (see Chapter 10); or a thin layer of 8 mm exposed aggregate (also see Chapter 10).
- 31. Surface slab systems 9 Table 2.2 German standard URC pavement design options [4] Layer thickness (mm) URC slab, 40 MPa compressive strength, 350 kg/m3 cement, 0.38 : 0.44 water–cement ratio, 4% entrained air content Cement bound base, 15 MPa compressive strength, pre-cracked (see Chapter 3) Crushed aggregate base Frost protection blanket 260 270 300 150 Membrane over 150 na 480 na na 490 300 300 Note na: not available. Linear cracking, divided slab or longitudinal crack Corner break Figure 2.2 Typical structural failure in URC pavements. URC modes of failure URC pavements typically fail by some form of tensile fatigue cracking. Further information on pavement failures may be obtained from references [5] and [6]. Repetitive tensile strains within the pavement structure eventually produce pavement surface cracks. The commonest forms of cracking are corner breaks and longitudinal cracks. Figure 2.2 illustrates the typical crack patterns found in a URC pavement. The cracking patterns determine the elements required in a URC pavement design method. 2.3 Jointed reinforced concrete (JRC) pavements JRC pavements are frequently constructed in a similar manner to URC pavements, in that a conventional longitudinal and transverse joint system is used, but reinforcement is added into the concrete. Figure 2.3 illustrates a typical stylised construction. The reinforcement provides two functions; it controls cracking and holds the joints tightly closed but can also instil additional
- 32. 10 Surface slab systems e d a b h i f g Key a transverse reinforcement b longitudinal reinforcement c support platform d trowelled border e pavement surface finish f tie bar (longitudinal joint) g dowel bar (transverse joint) h slab thickness i de-bonding membrane c Figure 2.3 A typical JRC pavement. Table 2.3 Maximum joint spacing for JRC pavements [1] Long slab systems Maximum transverse joint spacing Maximum longitudinal joint spacing Expansion joints Short slab systems Maximum transverse joint spacing Maximum longitudinal joint spacing Expansion joints 25 m 6m Every third transverse joint 10 m 6m Not required stiffness into the concrete slab. Reinforced concrete slabs can be constructed as either long or short slab systems (Table 2.3). Long slabs are constructed to a maximum length of around 25 m between transverse joints but typically require expansion joints (see Chapter 9) at each third joint. Short slab systems are constructed up to 10 m long between transverse joints but expansion joints are not usually required. A disadvantage of reinforced slabs is that the wider joint spacing precludes the use of plain joints. The wider transverse joint spacing produces larger thermal movements (as temperature increases and decreases) resulting in increased joint movement when compared with
- 33. Surface slab systems 11 URC pavements. These movements can only be accommodated using dowel bars or tied joints. The joint opening would be too large for plain joints. Reinforced systems can be designed as either cracked or uncracked slabs. Reinforcement is typically restricted to a single layer placed at mid-depth in the slab although some designers use separate top and bottom reinforcement. The typical highway standard reinforcement detail is to use 16 mm high tensile bar longitudinal reinforcement of between 500 mm2 and 1,000 mm2 /m2 of sectional area with nominal 12 mm diameter bars at 600 mm centres in the transverse direction. A frequently used standard form of industrial hardstanding is to use sheets of A393 (393 mm2 /m length in Grade 460 steel) mesh both at the top and bottom of the slab. A distinct advantage of ﬁxing the reinforcement in the centre of the slab is that the positive and negative moments are equally balanced thus allowing the slab to ﬂex equally before cracking and failing. The absolute minimum thickness of a reinforced concrete slab designed for trafﬁcking is 150 mm, although 200 mm tends to be a more generally accepted minimum, partly a function of the practical problems involved in providing adequate cover to the reinforcement. Reinforced concrete slabs are generally constructed across plastic de-bonding membranes but bituminous sprayed membranes may also be used. Reinforced concrete slabs are frequently used in place of mass concrete when: • • • workmanship and materials are suspect; the pavement could be subjected to large unplanned loadings; subgrade strength is weak or ill-deﬁned. JRC applications Bangkok city streets: short slab JRC system One of the best examples of the efﬁcient use of reinforced concrete can be found in the city streets of Bangkok. The streets are subjected to a very aggressive trafﬁcking regime in a very hot tropical climate. The city is also subject to subgrade problems that make the effective operation of bituminous pavements problematic. The city is built across a very low-lying river delta, frequently subjecting the streets to severe ﬂooding. Subgrade strengths are exceptionally low; a desiccated surface crust provides most of the strength. Ground water abstraction has also produced massive differential consolidation problems. Historically, poor workmanship has been a further major additional problem, and each of these contributory factors produces an exceptionally difﬁcult environment. But the reinforced concrete pavements operate effectively despite the extreme conditions. Pavements can be seen containing massive cracks, surface polishing and various forms of acid attack, but the system generally functions to an acceptable level of service despite the fact that very little planned maintenance is carried out.
- 34. 12 Surface slab systems A typical Thai pavement, will carry approximately 10 msa of trafﬁc and consists of: • • • • • • concrete surface brush ﬁnished; 250 mm JRC, 32 MPa 28-day characteristic compressive cube strength; longitudinal reinforcement 9 mm diameter at 170 mm centres, transverse reinforcement 9 mm diameter at 300–450 mm centres, all in low-grade plain steel bar; bay length 10 m, width one lane, with dowel and tie bar joints; plastic sheet de-bonding membrane; 150 mm crushed rock sub-base. Western European industrial sites Many small industrial sites are built with reinforced concrete slabs if designers lack conﬁdence that a mass concrete alternative would be constructed correctly. If small areas of concrete are required it is frequently preferable to use a reinforced slab and ensure that an unskilled labour force will successfully complete the project without any problems. A typical 10 msa pavement design consists of: • • • • • • • concrete surface brushed ﬁnish; 200 mm JRC, 40 MPa 28-day characteristic compressive cube strength, air-entrained concrete; A393 (393 mm2 /m in each direction) Grade 460 reinforcing mesh; bay size 10 m by 4–5 m, with dowels and tie bars; plastic sheet de-bonding membrane; 250 mm, 30% minimum soaked CBR, crushed rock sub-base; 5% CBR subgrade. JRC modes of failure JRC pavements crack and degrade in a similar manner to URC pavements with the exception that the pavement is more tolerant to cracking. Reinforced pavements are able to maintain a certain level of performance as cracking spreads through the structure. The additional integrity provided by reinforcement prevents a rapid deterioration of the pavement. JRC pavements frequently suffer from poorly placed reinforcement. Mesh sheets are frequently laid incorrectly supported by bricks or concrete spots resulting in a very poor standard of construction. Proper support chairs are needed to construct a successful pavement. US experience suggests that long slab systems are less reliable than short slab systems as they are more likely to suffer from mid-panel cracking,
- 35. Surface slab systems 13 joint sealant problems (due to greatly increased opening and closing) and consequent erosion of sub-base. 2.4 Continuously reinforced concrete (CRC) pavements CRC pavements are an extensively used form of construction employed on large motorway projects. This type of construction is typically economic if large quantities of sand, gravel and water are present on site. If these materials are available, CRC will be substantially cheaper than thick bituminous construction. Several different forms of construction are regularly found, of which the typical construction types are: Continuously reinforced pavement (CRCP in UK terminology), 100 msa design • • • • • • • 200 mm CRCP, 40 MPa 28-day characteristic compressive cube strength, surface running slab; reinforcement, 0.6% by section area, using 16 mm diameter high tensile, Grade 460 deformed bar and nominal transverse reinforcement in 12 mm bar; tied longitudinal joints (assuming the pavement is wider than 5 m); bituminous sprayed de-bonding membrane; 150 mm lean-mix concrete, 10 MPa 7-day mean compressive cube strength; prepared construction platform; the pavement ends are anchored into ground beams. Continuously reinforced roadbase (CRCR in UK terminology), 100 msa design • • • • • • • 100 mm bituminous surfacing; 150 mm CRCR, 40 MPa 28-day characteristic compressive cube strength; longitudinal reinforcement, 0.3% by section area, in Grade 460 deformed bar; bituminous sprayed de-bonding membrane; 150 mm lean-mix concrete 15 MPa 7-day mean compressive cube strength; prepared construction platform; note: no ‘anchorages’ are used with CRCR systems. The CRCP system can, if required, be surfaced with a 35 mm bituminous wearing course; the wearing course is not considered to contribute to the pavement strength.
- 36. 14 Surface slab systems Some US states use a double mat reinforcement system; the reinforcement mats are placed as top and bottom layers. The two layer system is used to avoid shear failures. The system can produce shear failures, along the plane of maximum shear, across the centre of the slab. A CRC pavement essentially consists of a regular pattern of cracked square plates connected together by steel reinforcement and aggregate interlock (Figure 2.4). The correct cracking pattern is essential to the efﬁcient operation of the pavement system. Cracking occurs progressively as the concrete shrinks and contracts in response to changes in temperature. The shrinkage cracking has been noted as occurring progressively over the ﬁrst 100 days of pavement operation. Pavement cracking is controlled by: • • • • concrete tensile strength; concrete shrinkage and the aggregate coefﬁcient of thermal expansion; low coefﬁcients of expansion produce the most favourable cracking pattern; the amount and grade of reinforcement; concrete temperature at construction; low temperatures produce the best and tightest cracking patterns. It is accepted that the following criteria are desirable to ensure an efﬁcient pavement system: • • • a crack spacing of between 1 and 2 m; a maximum crack width of 1 mm; a maximum wheel-induced reinforcement stress of 75% of the steel’s ultimate strength. b a d e c Key a nominal transverse reinforcement b longitudinal reinforcement c bituminous membrane d 35 mm bituminous surface course (optional) e slab thickness f lean-mix concrete sub-base layer Figure 2.4 A typical CRC construction. f
- 37. Surface slab systems 15 The design of a CRC system is a balancing act; adjusting the percentage reinforcement with the coarse aggregate qualities, cement content and placement temperature to produce the most efﬁcient crack spacing. McCullough and Dossey [7] report that the single most important factor inﬂuencing cracking is the aggregate type. Winter placed, low coefﬁcient of expansion, limestone aggregate is noted as producing the most desirable cracking patterns. A recent UK paper [8] has reported a ﬂint aggregate pavement that failed within 5 years of opening. The high coefﬁcient of expansion of the ﬂint aggregate as well as the omission of transverse reinforcement led to a rapid failure of the pavement. For CRCP, the required quantity of reinforcement is ﬁxed at around 0.6% of the sectional area in most design methods. The Belgian method uses 0.67% [9], the UK 0.6%; US methods ﬁx the rate at 0.65–0.67% [10]. It is noted that increasing the reinforcement percentage beyond these ﬁgures can produce poorly performing pavements [9]. A second important detail associated with CRCP construction is the need for ground anchorages at the ends of the CRC length. Two different forms of construction can be employed, a single rigid steel column detail or a system of reinforced concrete ground beams. Each of the anchorage details also includes expansion joints to allow some movement relative to the adjoining pavement construction. If a CRCP pavement is not provided with anchorages and joints, a large bump or ripple will occur at the start of an adjoining bituminous pavement. Chapter 10 contains details of the different anchorage designs. A thin bituminous 35 mm wearing course is currently considered the most practical UK form of surface ﬁnish, overcoming perceived noise and ride quality issues associated with concrete running surfaces. The wearing course is held in place using a bituminous pad coat. The main concrete slab can then be constructed in non air-entrained concrete. CRC applications CRC pavements are particularly useful for long continuous pavement construction carrying regular heavy trafﬁc loads. European motorway projects There is a long history of Western European motorway and large dual carriageway projects successfully constructed using this form of construction. The most notable recent UK application is a 30 km section of the recently constructed Birmingham Northern Relief Road (M6 Toll) project, which had the following construction: • 35 mm of 14 mm aggregate, negative texture thin surface course with a 1.5 mm minimum surface texture depth;
- 38. 16 Surface slab systems • • • sprayed bituminous emulsion bond coat, 0.8 l/m2 ; 220 mm CRCP, 40 MPa 28-day cube compressive strength; longitudinal reinforcement, 0.6% by section area, using 16 mm diameter Grade 460 deformed bar and nominal transverse reinforcement in 12 mm bar; bituminous sprayed de-bonding membrane; 200 mm lean-mix concrete, 10 MPa mean 7-day compressive cube strength; 5% CBR subgrade; pavement ends anchored into ground beams with expansion joints. • • • • A similar Dutch standard design permits the following construction: • • • • • • • 50 mm negative texture surface course; sprayed bituminous emulsion tack coat, 2 layers at 0.3 l/m2 ; 250 mm CRC, 45 MPa 28-day compressive strength; longitudinal reinforcement, 0.7% by section area, using 16 mm diameter high tensile deformed bar and nominal secondary reinforcement in 12 mm bar at 700 mm centres, set at 60◦ to the longitudinal reinforcement; 60 mm asphalt course; 250 mm crushed rock or cement bound sub-base; pavement ends anchored into ground beams with expansion joints. Airﬁeld runways John Lennon Airport runway in Liverpool, UK, was constructed using continuously reinforced concrete techniques and is a notable example of a successfully completed project. CRC modes of failure A good summary of current knowledge on modes of distress in CRC pavements can be found in [7] and [10]. The papers describe the following mechanisms: • • • • punch-outs; resulting from cracking which is too closely spaced; crack spalling; steel rupture across transverse cracks, resulting in the formation of wide cracks; steel corrosion.
- 39. Surface slab systems 17 Tayabji [10] summarises the following important characteristics for a low maintenance pavement: • • • • • high concrete compressive strength; cement treated base layer; longitudinal reinforcement of at least 0.59%; average crack spacing of 1–1.8 m; maximum crack width of 1 mm. It is accepted that pavement failure occurs progressively as cracking becomes more extensive and crack widths increase until the structural integrity of the pavement is lost. A heavily cracked pavement, with cracks spaced closer than 0.9 m, then becomes susceptible to punch out shear failures. 2.5 Variant slab systems Fibre reinforced concrete Steel ﬁbres represent an hybrid alternative to conventional reinforcement. They typically comprise thin strips between 30 and 70 mm in length and are dispersed into the concrete mix during production. Figure 2.5 illustrates typical ﬁbre shapes. Once the concrete layer is placed, the ﬁbres form a continuous reinforcement throughout the slab, the orientation of individual ﬁbres being essentially random. It is not generally economic to include sufﬁcient ﬁbre content for use as CRC – 0.5% by volume is a typical maximum ﬁgure – but ﬁbre reinforced concrete slabs are commonly used as JRC in industrial ﬂoor slab applications, the beneﬁt being the combination of wide joint spacing (particularly for internal applications where temperature variation is limited) and ease of handling (no reinforcement ﬁxing required). Figure 2.5 Typical shapes used for reinforcing ﬁbres.
- 40. 18 Surface slab systems Table 2.4 Typical UK pavement designs; 40 MPa strength [1] Trafﬁc level (msa) URC (mm) JRC (mm) CRCP (mm) A393 mesh reinforcement 16 mm Grade 460 0.6% 3% CBR at formation, 250 mm crushed rock sub-base 1 150 150 10 210 190 50 270 260 100 320 300 1,000 na na 3% CBR at formation, 250 mm crushed rock sub-base 1 150 150 10 180 170 50 240 230 100 270 270 1,000 na na 200 200 200 210 310 200 200 200 200 290 Note na: not available. A saving in thickness in comparison with the mass concrete (URC) alternative is also reported by some authors. 2.6 Summary Each of the different forms of construction can be used for numerous different applications but essentially the following applications are some of the most widely used (Table 2.4): URC JRC CRCP 2.7 Airﬁeld aprons, taxiways and runways, heavily trafﬁcked highway pavements in tropical countries; Industrial hardstandings, highway pavements in areas of low or uncertain subgrade strength; Motorway pavements on sites with large quantities of site won aggregates. References 1. The Highways Agency, Design Manual for Roads and Bridges, vol. 7, HD 26/01 ‘Pavement Design’, 2001. 2. Property Services Agency, A Guide to Airﬁeld Pavement Design and Evaluation, HMSO, 1989, ISBN 0 86177 127 3. 3. Petrie, E., Heavy duty concrete roads the Australian experience, Britpave Symposium, UK, October 2001.
- 41. Surface slab systems 19 4. Springenschmid, R., Recent development in design and construction of concrete pavements at German Expressways (Autobahns), 7th International Conference on Concrete Pavements, September 2001. 5. Shahin, M.Y., Pavement Management for Airports, Roads and Parking Lots, Chapman and Hall, ISBN 0-412-99201-9. 6. Burks Green and Highways Agency, Concrete Pavement Maintenance Manual, The Concrete Society, ISBN 0 946691 89 4. 7. McCullough, B.F. and Dossey, T., Controlling early-age cracking in continuously reinforced concrete pavement, Transport Research Report 1684, Washington DC, January 1999. 8. Cudworth, D.M. and Salahi, R., A case study into the effects of reinforcement and aggregate on the performance of continuously reinforced concrete pavements, 4th European Symposium on Performance of Bituminous and Hydraulic Materials in Pavements, BITMAT 4, Nottingham, UK, April 2002. 9. Verhoevan, K., Cracking and corrosion in continuously reinforced concrete pavements, 5th International Conference on Concrete Pavement Design and Rehabilitation, Purdue University, April 1993. 10. Tayabji, S., Performance of continuously reinforced concrete pavements in the LTPP program, 7th International Conference on Concrete Pavements, September 2001.
- 42. Chapter 3 Concrete bases and sub-bases 3.1 Introduction The foundation beneath a pavement is frequently constructed in either a low strength cracked cement bound material or a higher-quality concrete material. UK practice is to construct heavily trafﬁcked URC, JRC and CRCP pavements across high-quality cement bound materials, the high-quality material providing support to the surface slab system. High-quality cement bound materials can also be used with bituminous materials to form ﬂexible composite pavements. Lower-quality sub-base materials are also used with bituminous pavements but their lack of tensile capacity reduces the structural value of the material. Flexible composite (or semi-rigid) pavements are distinctly different to surface slab systems in that they obtain their strength from a combination of the structural capacity of the bituminous and cement bound layers. Three different groups of structures can be identiﬁed: • • Roller compacted concrete (RCC) systems: RCC is principally used in the US and is a strong cement bound material (typically 40 MPa compressive strength) generally used as a complete pavement structure. The material is batched then laid semi-dry using a paver. Cracks are frequently induced as part of the construction process (see Chapter 9). In low-speed applications (ports, industrial areas, estate roads), RCC can actually form the surface; otherwise, a bituminous surface course would be added. Cement bound material (CBM) base systems (known hereafter as ﬂexible composite systems): these are true ﬂexible composite pavements and involve a substantial bituminous bound layer working in association with a structurally signiﬁcant cement bound layer (typically 10–20 MPa compressive strength). Roller compacted lean-mix concrete is generally used for the cement bound layer, with cracks formed as detailed in Chapter 9.
- 43. 22 Concrete bases and sub-bases • CBM sub-base systems: these pavements consist of low-strength CBM, with a thick bituminous layer acting as the main structural member in the pavement system. The CBM acts as a granular sub-base. Figure 3.1 describes a typical sketch comparing the three alternative pavement types. The choice as to whether a pavement should be considered as true ﬂexible composite or a CBM sub-base system is often not clear cut; the South African standard [1] suggests that it is a function of how the pavement layers are ‘balanced’. An alternative explanation would be to suggest that the bituminous and CBM materials will, at the start of the pavement life, carry certain proportions of the load. If the CBM layer is loaded beyond the tensile fatigue capacity of the material, cracking occurs and the CBM layer deteriorates. The cracked layer then begins to act in a similar manner to a conventional crushed rock or granular layer and the bituminous layer carries a higher proportion of the load. It can therefore be concluded that the choice between ﬂexible composite and CBM sub-base is a function of: • • • • • the magnitude of the wheel load; thickness of overlying bituminous material; CBM material strength and structural capacity; environmental conditions; the degree of cracking introduced into the CBM layer during the construction process. A ﬂexible composite pavement works as a bonded system with substantial tensile stress taken by the CBM layer. CBM sub-base systems may begin life as bonded systems but the weaker CBM layer quickly degrades down into a cracked, broken layer similar to a crushed rock. In all of these pavement types, relatively low-strength CBM can also be used within the pavement foundation, sometimes resulting in two or three consecutive cementitious layers separating the bituminous surfacing from the subgrade. 50 mm Asphalt 225 mm 40 MPa RCC RCC 180 mm Asphalt 250 mm Asphalt 250 mm 15 MPa CBM 200 mm 4.5 MPa CBM Flexible composite Figure 3.1 Approximately equivalent composite systems. CBM sub-base system
- 44. Concrete bases and sub-bases 3.2 23 Roller compacted concrete (RCC) systems The simplest form of construction is the US practice of using RCC pavements. The system is a very simple one in which a semi-dry concrete is laid and compacted in a single layer. The system is summarised in a Portland Cement Association (PCA) paper [2]; essentially it involves the following works: • • • A 12% cement content non-air-entrained silica fume OPC blended mix of semi-dry concrete is batched then laid through a paver. A typical highway pavement slab is 225 mm thick. The concrete is compacted to give a very high density. Rollers are used to achieve the ﬁnal closed surface of the RCC layer. A typical ultimate, cored in situ compressive strength will be 40 MPa. Joints are frequently formed naturally but in more modern systems sawing or notching is used to create formed joints. The joints are seldom sealed. The pavement surface can, where required, be ﬁnished with a 50 mm layer of Asphalt surface course. Reﬂective cracks are allowed to form through the Asphalt layer. Industrial sites are frequently left unsurfaced. RCC applications The PCA paper [2] notes that the system is extensively used in North America; it is used as an alternative option in many major schemes. The pavements are typically used for: • • • freight terminals; storage yards; minor low-speed rural roads. The following typical pavements are reported: • • • container yards equipment storage minor highways 450 mm RCC, exposed surface 300 mm RCC, exposed surface 50 mm Asphalt overlay over 225 mm RCC base. RCC modes of failure The PCA report [2] fails to describe a manner of failure but it must be assumed that the material will deteriorate in a similar manner to all surface slab systems. The pavements will deteriorate by fatigue cracking which, if bituminous materials are present, will then reﬂect to the surface.
- 45. 24 3.3 Concrete bases and sub-bases Flexible composite systems Flexible composite pavements are frequently used in place of conventional bituminous construction in situations where substantial quantities of site won aggregates can be commercially exploited, reducing the demand for bitumen and crushed rock aggregate. However, they can be more difﬁcult to construct than conventional systems; the bituminous layers must also be placed and compacted without introducing excessive cracking in the CBM base layer. Flexible composite applications A typical UK 20 msa ﬂexible composite motorway pavement design [3] will consist of: • • • • • • 190 mm bituminous surfacing; 250 mm CBM, crushed rock aggregate, CBM3R well controlled grading, 10 MPa mean 7-day compressive cube strength; 150 mm CBM, aggregate and grading much less tightly controlled, CBM2A 10 MPa mean 7-day compressive cube strength; CBM layers paver-laid, semi-dry condition, pre-cracked at 3 m centres; 250 mm granular or stabilised capping, 15% CBR; 5% CBR subgrade. In the airﬁeld industry, it is common to use multi-layer CBM base beneath a bituminous surfacing. In effect, the combined CBM and bituminous layers are assumed to act together in protecting the underlying subgrade from the often very substantial load from an aircraft undercarriage. This can sometimes demand combined thicknesses of several hundred millimetres. The key decision, upon which not all airport experts agree, is the proportion of these bound layers which should be bituminous and the proportion which may be cement bound. In the UK it is standard practice [4] to insist that at least one-third of the thickness is bituminous, whereas US practice [5] is to permit as little as 125 mm of bituminous (100 mm for light aircraft). Logically, the issue is one of whether reﬂective cracking (the propagation of CBM cracks/joints through to the surface) is to be tolerated or not. If not, then most climates would probably demand at least 180 mm of bituminous surfacing. Flexible composite modes of failure Bonded ﬂexible composite pavements deteriorate by CBM fatigue cracking; as the CBM deteriorates de-bonding occurs. The de-bonded layers produce a weaker pavement. The South African [1] and French [6] design methods contain descriptions of how pavements deteriorate. The standards suggest that immediately after construction the pavement acts as a fully bonded
- 46. Concrete bases and sub-bases 25 system, the bituminous materials and each layer of CBM is considered to act together producing a single elastic slab response. Initially the CBM layer is assumed to carry most of the load. The ﬁrst mechanism of deterioration is considered to be fatigue cracking of the CBM layer. Cracking then begins in the de-bonded bituminous surface and subgrade deterioration may also then occur. The stiff uncracked CBM layer is the most structurally signiﬁcant element in the pavement and acts as the main structural support member; when the CBM layer begins to deteriorate the structural capacity of the system is substantially reduced. In practice reﬂective cracking is ﬁrst noted, since the CBM tends to break into large discrete ‘blocks’. Producing stress in the overlying bituminous material. The South African standard [1] suggests that the long-term structural response of the pavement is a function of the state of the structure within the deterioration process. The ﬁnal stage of deterioration is observed when the CBM layer acts in a similar manner to a granular sub-base system. South African and French researchers suggest that ﬂexible composite pavements are brittle when compared with bituminous and granular systems. Figure 3.2 describes a typical section through a ﬂexible composite pavement and describes the point where maximum stress occurs. 3.4 CBM sub-base systems Cement bound sub-base systems are in many ways similar to ﬂexible composite pavements, the essential difference being that the CBM layer acts in Wheel load 2 Bituminous layer strain, fatigue cracking Bituminous layer CBM layer CBM layer Subgrade 1 CBM layer strain, fatigue cracking; designed using uncracked CBM stiffness 3 Subgrade strain; used to predict permanent deformation (i.e. rutting) Figure 3.2 Deterioration of a ﬂexible composite pavement.
- 47. 26 Concrete bases and sub-bases a manner similar to a granular sub-base. The South African standard [1] suggests that two different classes of CBM sub-base can be produced: • • Strong systems, which act as superior granular materials and will have an approximate apparent modulus of 300–500 MPa (compared with 200–300 MPa for most granular bases). Weak systems, from lower-quality aggregate mixes, producing a modulus of 100–200 MPa. CBM sub-base system applications The South African Standard [1] contains a number of examples of cement bound sub-base designs. A typical South African main highway pavement designed to carry 3 msa consists of: • • • • • • 30 mm Asphalt surfacing; 150 mm CBM Grade C3, 1.5–6.0 MPa compressive strength; 200 mm CBM Grade C4, 0.75–1.5 MPa compressive strength; 150 mm granular material Grade G7, 15% CBR; 150 mm granular material Grade G9, 7% CBR; Subgrade, minimum CBR 3%. The standard also contains extensive lists of other possible ﬂexible composite pavement design options. The French and American standards contain similar examples. The UK experience of CBM sub-base systems essentially exchanges crushed rock for CBM material. The UK sub-base systems have historically made use of CBM with 7-day mean compressive cube strengths of either 4.5 or 7 MPa. New designs taking account of the different possible strengths of pavement foundation resulting from the use of different sub-base materials, are currently in preparation. CBM sub-base systems modes of failure This type of pavement effectively behaves as a fully ﬂexible structure and therefore has modes of deterioration typical of such pavements, namely bituminous material fatigue cracking and rutting, together with the possibility of subgrade deformation. An important factor that is frequently misunderstood is the inﬂuence of adverse environmental effects on the durability of CBM materials. CBM sub-base systems can be affected by acid attack, low pH ground water or sulphate attack which may contribute to a lower than expected effective stiffness for the layer. A number of UK examples exist of adverse ground conditions substantially reducing the durability and strength of CBM sub-base systems. This issue would beneﬁt from further investigation. Regrettably no
- 48. Concrete bases and sub-bases 27 speciﬁc published guidance exists linking chemical attack to CBM material speciﬁcations. 3.5 Summary Roller compacted concrete, ﬂexible composite and CBM sub-base systems can offer substantial ﬁnancial and environmental advantages when compared with more traditional alternatives. The most important fact is that they can be used as direct replacements for conventional crushed rock or bituminous materials, allowing signiﬁcant reductions in cost and environmental impact. Substantial reductions in the thickness of a bituminous layer can be achieved if correctly designed and constructed CBM layers are used in place of crushed rock sub-base systems. These types of pavement are most economically and successfully used in the following applications: • • • 3.6 roller compacted concrete – Industrial hard-standings or low-speed roads in areas with readily available hard aggregates; f lexible composite pavements – high-speed, high-quality highways and airﬁelds, especially when site won aggregates are available; CBM sub-base applications – any roads where large quantities of lowquality or marginal sand aggregates are available. References 1. Committee of Land Transport Ofﬁcials COLTO, Structural Design of Flexible Pavements for Interurban and Rural Roads, Draft TRH4, Pretoria, South Africa, 1996, ISBN 1-86844-218-7. 2. Piggott, R.W., Roller compacted concrete pavements – a study of long term performance, Portland Cement Association, Illinois, RR366, 2000. 3. The Highways Agency, Design Manual for Roads and Bridges, vol. 7, HD 26/01 ‘Pavement Design’, 2001. 4. BAA plc, Group technical services aircraft pavements, pavement design guide for heavy aircraft loading, R. Lane, 1993. 5. International Civil Aviation Organisation, Aerodrome Design Manual, Part 3 Pavements, 2nd edn, 1983. 6. Laboratoire Central de Ponts et Chaussées, French Design Manual for Pavement Structures, Service d’Etudes des Routes et Autoroutes, 1997, D 9511TA 200 FRF.
- 49. Chapter 4 Testing and speciﬁcation 4.1 Introduction A concrete pavement design method must include a number of elements to successfully complete a pavement design. • • • Index testing of the bound materials to measure and control strength. A fatigue model and an accepted set of relationships linking the index test results back to a calculation technique. A standard recognised speciﬁcation to classify materials and set acceptance limits to deﬁne when materials may be successfully employed within the pavement. Each of these elements is examined within this chapter. 4.2 Standard strength test methods The measurement, description, testing and control of the concrete element within a pavement represents a signiﬁcant design problem. The stiffness and condition of the material within the pavement is difﬁcult to estimate. It is well understood that the strength of concrete increases with time but pavement material strength cannot be directly measured in situ by any of the available test methods. However, a number of different laboratory methods may be employed to test concrete strength (refer to Figure 4.1) and each test is described within this section. It is noted that none of the tests precisely replicates the exact conditions that occur in the pavement. Pavement material strength may therefore be estimated but never precisely measured.
- 50. 30 Testing and speciﬁcation Compressive tests Cylinder F Cube Indirect tensile splitting tests F Hardboard Cube length l, depth d Cylinder length l, diameter d F/2 F/2 Flexural beam test d depth by b width L L L Figure 4.1 Strength testing of concrete samples. Compressive cylinder (or core) strength Compressive cylinder tests form the most extensively used method of strength control. The essential features of the test are: • • The size of the sample is controlled; standard cylinders are 150 mm diameter by 300 mm long, although tests may be carried out on any cylinder with a length to diameter ratio between 1 and 2. Cylinders may be produced from moulds ﬁlled with pavement concrete or cores taken from the completed pavement.
- 51. Testing and speciﬁcation • • • • 31 The method of sampling, compaction and curing is controlled. The test is conducted on wet samples. The rate of compressive strain application is controlled. The rate of reproducibility is around 13%. The test may be used to measure in situ pavement strength from cores taken out of the pavement. Compressive cylinder strength is accepted as a representative measure of ultimate compressive strength. Compressive cube strength The compressive cube strength test forms the basis of UK concrete strength control. Cubes are used in preference to cylinders as they are smaller, easier to store and can be made relatively simply. Two different sizes are regularly used, 100 and 150 mm. Results from both sizes are considered of equal value. Compressive cube strengths are higher than cylinder strengths. When a concrete cube is compression tested the cube’s geometry produces a conﬁned testing condition. The steel platens on the compression testing machine restrain the concrete cube at failure and produce higher compression test results when compared to cylinder tests. The essential features of the compressive cube strength test are: • • • • • The method of sampling, compaction and curing is controlled. The test samples must be wet when tested. The compression-testing machine must have a controlled rate of strain application. The 100 mm test is considered to have a 15% reproducibility coefﬁcient. The 150 mm test is slightly more precise having a 13% reproducibility. Compressive cube strength can be related to cylinder strength. CEB-FIP Model Code 90 [2] gives values for equivalent compressive cylinder and cube strengths. fc,cyl fc,cube 12 15 20 25 30 37 40 50 50 60 60 MPa 70 MPa A well-known empirical relationship is used to link cube and cylinder strength, cylinder strength is approximately equal to 80% of cube strength. Axial tensile strength The axial tensile test is a measure of true tensile strength but the test is not generally accepted as a practical method of control in a construction
- 52. 32 Testing and speciﬁcation speciﬁcation. The test is essentially a research tool but will produce the most accurate measure of tensile strength. The test is carried out on standard cylinders; tension is applied from either glued end plates or radial scissor grip side clamps. A preliminary draft European norm, prBS EN 13286-40 [1] exists, based primarily on French experience. Indirect tensile splitting strength As an alternative, the indirect tensile (or Brazilian) splitting test is extensively used to assess tensile strength. The test is well known, deﬁned and controlled, but many authorities consider that the test is not a suitable measure of tensile strength. The test is conducted by applying a line load across the diameter of a concrete cylinder (or to the surface of a cube). The essential features of the test are: • • • • • It is usually conducted on cylinders but the UK standard permits the use of cubes. Cylinders are loaded through 15 mm by 4 mm hardboard strips, cubes through similar but smaller areas (6 mm square for 150 mm cubes, or 4 mm square for 100 mm cubes). The test is conducted using a standard compression-testing machine and the rate of strain application is controlled. The test has an 18% reproducibility coefﬁcient. The splitting stress is estimated by assuming that failure occurs across the central two-thirds of the failure plane, resulting in the following equation. Equation 4.1 Tensile splitting strength ft,sp = 2F πld (4.1) ft,sp = tensile splitting stress F = applied force l = cylinder or cube length d = cylinder diameter or cube length CEB Model Code 90 [2] suggests that a direct relationship exists between ultimate axial tensile strength and tensile splitting strength. Equation 4.2 Tensile splitting strength to tensile axial strength after [2] ft,sp = 0.9 ft,axl (4.2) Various attempts have been made to relate tensile splitting strength to compressive strength; Oluokun et al. [3] presents a relationship.
- 53. Testing and speciﬁcation 33 Equation 4.3 Tensile splitting strength to cylinder strength after Oluokun et al. [3] ft,sp = 0.214 fc,cyl 0.69 (4.3) An important UK paper rejects these hypotheses and strongly asserts that the tensile splitting test is incorrectly considered to be a measure of tensile strength. BRE Digest 451 [4] notes that a substantial indirect tensile strength may be obtained by conducting the test on pre-split cylinders. If a cylinder is cut along the line of the expected failure plane it is still possible to obtain 50% of the split strength. The Digest notes that the test is a form of shear test; recording the possible shear strength of a concrete rather than the true axial tensile strength. It should be noted that indirect tensile tests can also be used to measure Young’s Modulus, following a similar procedure to that commonly used for Asphalt [5]. Young’s Modulus, though not generally used in speciﬁcation, forms an important input to certain pavement design methods. The equation which applies is as follows and is an uncracked E dynamic: Equation 4.4 Young’s Modulus [5] derived from ITSM testing E= F (0.273 + ν) h·l (4.4) E = Young’s Modulus h = horizontal diametral extension Other quantities are as deﬁned previously Flexural strength (or modulus of rupture) The ﬂexural beam test (see Figure 4.1) is frequently used as a method of evaluating tensile strength for concrete pavement design and is generally accepted as the most representative test for assessing the tensile capacity of concrete pavement materials, since it is considered to establish the extreme ﬁbre tensile strength in bending. A development of the test is also used to estimate the ultimate strength and the toughness of ﬁbre reinforced concrete. The essential features of the test are: • • • • • • The depth of the beam (d) is generally equal to the width (b). The beam length is between four and ﬁve times the depth. The ratio of d (or b) to maximum aggregate size should not be less than 3. Specimens may be either beams sawn from the pavement or prisms manufactured and cured in accordance with the relevant standard. Test specimens must be wet. The test has a similar level of repeatability to the tensile splitting test and has an 18% reproducibility.
- 54. 34 Testing and speciﬁcation • The British Standard test [6] allows compression testing of the discarded beam-ends thus producing a direct relationship between ﬂexural and compressive cube strength. The equation for ﬂexural strength is as follows: Equation 4.5 Tensile ﬂexural strength ft,f l = FL (4.5) bd 2 ft,f l = tensile ﬂexural strength (known as ‘modulus of rupture’ in the USA) F = applied load L = distance between supporting rollers d = beam depth b = beam width Link between axial and tensile strength It can clearly be seen that the ultimate stress calculated from the beam test is not the true tensile capacity of the concrete. Figure 4.2 illustrates the fact that at failure extreme ﬁbre yield occurs before the sample fails. The axial tensile fl Strain/stress measured on the surface of the slab ft A Strain/stress assumed in a flexural test or bending in a mass concrete slab A Mass concrete beam in bending Neutral axis A Stress/strain plot along AA ft A fl Figure 4.2 Bending stress/strain in a mass concrete beam.
- 55. Testing and speciﬁcation 35 capacity of the concrete therefore turns out to be a function of the test sample size. The ultimate bearing capacity of a mass concrete section is therefore a function of the pavement thickness. This increase in ultimate capacity in a thick concrete pavement is rarely used in design. Most pavement design methods use the allowable ultimate stress as a function of the ﬂexural beam strength. The CEB code [2] suggests a relationship (Equation 4.6) linking axial tensile capacity to a ﬂexural beam strength. The relationship offers an interesting adjustment to the commonly accepted ﬂexural test based fatigue model. The model gives reasonable results on pavement thicknesses between 100 and 250 mm, but will underestimate ultimate strength in pavements thicker than 250 mm. Equation 4.6 Flexural strength to axial strength relationship after [2] ft,axl = ft,ﬂ 1.5 hb /0.1 0.7 1 + 1.5 hb /0.1 0.7 (4.6) ft,axl = mean tensile axial strength fﬂ = ﬂexural stress at failure hb = slab thickness In the case of 150 mm deep beams, Equation 4.6 reduces to a factor of 0.67 between ﬂexural stress at failure and axial strength. For 100 mm deep beams, this factor becomes 0.6. Strength for pavement design and construction control In order to successfully complete the design of a pavement it is essential to understand several key features associated with the estimation of a pavement’s true bearing capacity. The key features are, in order of importance: • • • the relationship between ﬂexural strength (used in design) and compressive strength (used to control concrete manufacture). the estimation (or measurement) of the uncracked Young’s Modulus, generally based on compressive strength. the fatigue model used within design. Furthermore the following issues are of key importance in relation to environmental effects on pavement life: • • the thermal expansion coefﬁcient. concrete durability.
- 56. 36 Testing and speciﬁcation This section will discuss the issue of concrete strength for pavement design. Sections 4.4–4.7 will address the remaining issues. Flexural strength to compressive strength relationships The relationship linking a compressive strength to a ﬂexural strength, and therefore to an axial strength, is not ﬁxed. It is well known and recorded that the link between the expressions is a function of: • • • • coarse aggregate quality; coarse aggregate type (gravel or crushed rock); cement type, quantity and quality; cleanliness of the ﬁne aggregate. The following general expression linking compressive cube strength and ﬂexural strength is given in Technical Report 34 [7]. Equation 4.7 General cube strength to ﬂexural strength relationship [7] ft,f l = 0.393fc,cube 0.66 (4.7) It is well known that river gravel can give a lower tensile to compressive strength ratio than crushed rock aggregate. Croney and Croney [8] gives two alternative relationships to link ﬂexural strength to compressive cube strength; it is probable the relationships are derived from high-strength, airentrained concrete. Equation 4.8 Compressive cube strength to ﬂexural strength after Croney and Croney [8] ft,ﬂ = 0.49fc,cube 0.55 ft,ﬂ = 0.36fc,cube 0.70 (for gravels) (4.8a) (for crushed rock) (4.8b) De Larrard [9] quotes similar relationships (Equations 4.9a and 4.9b) for different French aggregate sources. De Larrard’s testing was conducted using foil-cured specimens but generated similar relationships to that of Equation 4.7. They are particularly useful in comparing different possible aggregate sources. De Larrard probably used non-air-entrained concrete. Equation 4.9 Tensile splitting strength to compressive splitting strength after De Larrard [9] ft,sp = kt fc,cyl 0.57 (4.9a) ft,ﬂ = kt 1.44fc,cube 0.57 (4.9b)
- 57. Testing and speciﬁcation Key Marine ﬂint aggregate Hard limestone aggregate Semi-hard limestone aggregate Basalt aggregate Quartzite aggregate 37 kt = 0.442 kt = 0.344 kt = 0.365 kt = 0.445 kt = 0.398 Supporting data The following data, illustrated in Figure 4.3, was collected by the authors and broadly supports these ﬂexural strength to compressive strength relationships. Manchester airport, UK Coarse aggregate, Derbyshire limestone; OPC; 40 MPa 28-day compressive cube mix. fc,cube 28-day mean 57.81 MPa standard deviation 7.57 MPa 47.39 MPa standard deviation 6.32 MPa fc,cube 7-day mean 28-day mean 5.85 MPa standard deviation 0.67 MPa ft,ﬂ Coventry airport, UK Coarse aggregate, Leicestershire granodiorite; OPC; 40 MPa 28-day compressive cube mix. fc,cube fc,cube ft,ﬂ 28-day mean 58.73 MPa standard deviation 3.02 MPa 7-day mean 47.90 MPa standard deviation 3.25 MPa 28-day mean 6.00 MPa standard deviation 0.39 MPa 8 Flexural strength (MPa) 7 6 5 4 TR 34 [7] Croney and Croney [8] gravel Croney and Croney [8] rock De Larrard [9] limestone De Larrard [9] basalt 3 2 Manchester airport 1 Coventry airport Ryong, thailand 0 0 20 40 60 80 Compressive cube strength (MPa) Figure 4.3 Summary of compressive cube to ﬂexural strength data.
- 58. 38 Testing and speciﬁcation General motors site at Ryong,Thailand Coarse aggregate, granite; non-air-entrained; 40 MPa 28-day compressive cube mix. fc,cube ft,ﬂ 28-day mean 58.9 MPa standard deviation 3.44 MPa 28-day mean 5.26 MPa The two sets of available UK data suggest that the mean ﬂexural strength of a pavement mix is similar for different mixes produced using a standard speciﬁcation but the Thai data illustrates that the relationship will change for different concrete mix types. 4.3 In situ pavement compaction and strength The level of in situ compaction of a concrete will inﬂuence the ultimate strength of the pavement; basically the higher the level of compaction, the higher the pavement’s ultimate strength. The density and void content of cores taken from the pavement must therefore be monitored and controlled to ensure the concrete (or cement bound base material) will achieve a minimum level of compaction and therefore pavement strength. It should be noted that the core test will measure the total (entrained and other) void content within the concrete and that the greater the volume of entrained air within the concrete the lower the concrete strength will be. An important element within any design method is the estimate linking index strength tests to the actual achievable strength of the in situ concrete within the pavement, for which very little published data exists. The following approximate relationships can be used to link in situ strength to index testing results. • • 28-day standard tank cured strength = ultimate in situ strength. 28-day standard tank cured strength = 1.2 × 28-day in situ strength. Curing The precise and correct curing of cement bound materials is an important element contributing to the successful testing of samples. It is noted that all of the recognised testing methods deﬁne precise rules for curing concrete samples. The essential features of a curing regime are: • • • The samples must be kept for a speciﬁc time period within a controlled temperature water bath. The test water must be of a controlled quality. Tests are typically conducted at 7, 28 and 90 days.
- 59. Testing and speciﬁcation 39 CEB Model Code 90 [2] offers the following relationship to allow the estimation of test strength at key dates after the construction of a pavement. Equation 4.10 Relationship between strength and time from CEM Code 90 [2] β = exp S 1 − 28 T 0.5 (4.10) β = factor to adjust 28-day strength S = cement factor, 0.25 for normal and rapid hardening cement, 0.38 for slow hardening cement. T = number of days since construction Equation 4.10 suggests that the 28-day strength can be factored using the following coefﬁcients for OPC mixes. 7-day strength = 0.78 × 28-day strength 90-day strength = 1.12 × 28-day strength 360-day strength = 1.20 × 28-day strength Young’s Modulus for uncracked concrete The stiffness or Young’s Modulus of an uncracked cement bound material cannot be easily directly measured. Standard relationships linking stiffness to strength are accepted as a realistic measure of stiffness. Several researchers have also used ultrasonic techniques to link stiffness density and static modulus. The ultrasonic test is simple to perform and is usually completed on a beam sample. The test will not directly measure stiffness but standard relationships linking ultrasonic speed of transmission to stiffness can be used. It is therefore usual to derive an approximate Young’s Modulus from strength test data. Standard practice is to assume a ﬁxed Poisson’s Ratio of 0.15 for static and 0.2 for dynamic pavement calculations and to estimate Young’s Modulus based on either compressive cube or cylinder strengths. The level of stress within a concrete pavement layer is usually designed to be relatively low, well below the ultimate strength of the material. It is therefore suggested that dynamic fatigue and strength calculations for pavement design are conducted with Young’s Modulus equal to the ‘Initial Tangent’ value. The Initial Tangent value is the true elastic modulus, free from the effects of creep or yield. CEB Model Code 90 [2] recommends the following for design.
- 60. 40 Testing and speciﬁcation Equation 4.11 Tensile splitting strength to tensile axial strength after [2] Eci = 21.5C fc,cyl 0.333 10 × 106 GPA (4.11) Eci = Initial Tangent Young’s Modulus for dynamically loaded uncracked material C = correction factor, as follows: 1.2 for basalt or dense limestone 1.0 for quartzite 0.9 for standard limestone 0.7 for sandstone The initial creep-free Young’s Modulus is not commonly used in structural engineering; most structural engineering calculations use the value adjusted to the ‘Secant Modulus’, Ec , which the CEB-Code [2] suggests is 0.85 of the Initial Tangent Modulus. Statically loaded pavements such as warehouse ﬂooring should be treated slightly differently. The long-term modulus is signiﬁcantly different to the short-term value. Speciﬁc creep-adjusted values may be estimated but the long-term value may reasonably be taken as twothirds of the Initial Tangent value. Equation 4.12 Young’s Modulus values [2] Eci = 1.18Ec = 1.5Elong-term (4.12) Eci = dynamic uncracked Young’s Modulus (Initial Tangent Modulus) Ec = static uncracked Young’s Modulus (Secant Modulus) Elong-term = long-term static uncracked Young’s Modulus 4.4 Concrete fatigue A concrete fatigue model is an important element linking together index test results and the structural capacity of the pavement. It is well understood that repeated loads produce tensile stresses which then induce concrete cracking and pavement failure. Pavement life is linked to the magnitude of stress in relation to concrete strength. The difﬁculty in design is knowing how to link estimated stresses to the number of load cycles which induce failure, and then producing a reliable estimate of pavement life. It is generally accepted
- 61. Testing and speciﬁcation 41 that the following factors are directly related to concrete fatigue capacity: • • • • • frequency of loading and amplitude of the loading cycle; moisture condition; age of the concrete; stress condition and stress gradient; quality and composition of the concrete. None of these effects can be precisely calculated or measured. Basis of fatigue models The relationship between the number of load repetitions producing a tensile stress, and the ﬂexural strength, is linked using the ‘Miner’s Law’ principle; cumulative damage at different tensile stress levels is summed to produce an estimate of pavement life. A power law is used to relate the effects of stresses at different percentages of the ultimate strength. The power law is also used to link different axle loads back to a ‘design axle load’ and therefore to an estimated pavement life. Chapter 6 describes this relationship in more detail. Within the context of concrete pavement design, three different types of fatigue model may be found. All of the well-known fatigue models utilise the ﬂexural tensile strength at failure. Tensile splitting strength and axial strength are not generally used. The three main model types involve the following input variables: 1 2 3 ft,ﬂ , σt,ﬂ ft,ﬂ , σt,ﬂ , R ft,ﬂ , σt,ﬂ , R, t ft,ﬂ = ﬂexural tensile strength from the standard beam test σt,ﬂ = tensile stress calculated under a design load R = ratio maximum to minimum stress within the loading cycle t = duration of loading pulse Within the context of this document discussion is conﬁned to the simplest and most widely used form of model, involving simply ﬂexural strength and tensile stress under load. Further information on concrete fatigue models may be obtained from the paper by Stet and Frenay [10]. Laboratory fatigue data Numerous researchers have published fatigue data, usually from repeated load ﬂexural beam tests. In general, when the number of load applications
- 62. 42 Testing and speciﬁcation Concrete fatigue data and design models Allowable stress ratio to 28-day flexural strength 0.9 Beam test data Adjusted mean relationship (12) R = (16. 61–LogN)/17.61 0.8 PCA mean relationship (11) R = (17.61–LogN)/17.61 0.7 0.6 PCA design relationship (11) R = (11. 73–LogN)/12.077 0.5 US airfield data 0.4 PCA design relationship (11) R = ((4.2577/LogN)^0.306) –4.325 0.3 10 100 1,000 10,000 PCA design relationship (11) for long life R < 0.45 100,000 1,000,000 10,000,000 Number of repetitions to failure Figure 4.4 Fatigue data and design models. causing failure is plotted against the ratio of applied ﬂexural tensile stress to ﬂexural tensile strength, the data tends to group within a relatively narrow band. Figure 4.4 includes a set of ﬂexural beam test data. Note that a characteristic of concrete in fatigue is its extreme sensitivity to load level, illustrated by the shallow gradient of the lines in Figure 4.4, and for this reason it is prudent to ensure that a reasonably generous safety margin is designed into a pavement, in order to account for the uncertainties and variations that are inevitably present in such matters as concrete strength and foundation stiffness, not to mention as-constructed slab thickness. The Portland Cement Association model The most widely accepted commercial concrete fatigue model is the Portland Cement Association relationship developed by Packard and Tayabji [11]. The Packard model is a semi-empirical relationship linking Westergaard stresses (see Chapter 5) to the 28-day ﬂexural strength from beam tests. Different equations are given for 50% probability and for recommended design, the latter having a greater factor of safety. Darter and Barenberg [12] then proposed a slight adjustment to the relationship for the 50% probability case. It is noted that stress below 0.45 of the ultimate strength is considered to be non-damaging. Equations 4.13 and 4.14 give details of these relationships, which are also illustrated in Figure 4.4. Figure 4.4 also makes the point that the PCA expressions cannot be used to obtain a precise design.
- 63. Testing and speciﬁcation 43 Table 4.1 Summary of coefﬁcients of thermal expansion [13] Aggregate type Concrete thermal coefﬁcient (10−6 /◦C) Flint Quartzite Sandstone Gravel Granite Basalt Limestone 20 11.9 11.7 10.8 9.5 8.6 6.8 Equation 4.13 The PCA [11] fatigue design relationships R= R= R 11.73 − Log10 N 12.08 4.2577 Log10 N R > 0.55 (4.13a) 0.45 < R > 0.55 (4.13b) 0.306 − 0.4325 0.45 N =∞ (4.13c) Equation 4.14 The PCA [11] 50% probability relationship R= 16.61 − Log10 N 17.61 (4.14) R = the ratio of tensile stress to ﬂexural strength from the 28-day standard beam test N = the number of load repetitions to failure Concrete thermal coefﬁcient The expected temperature gradient through a pavement, leading to differential expansion and contraction and therefore warping, may have a signiﬁcant effect on the choice of joint design and on the fatigue life of a concrete. The coefﬁcient of thermal expansion is a function of the coarse aggregate type, cement content and humidity. The following coefﬁcients, presented in Table 4.1 as quoted in AASHTO [13] are suitable for pavement design. 4.5 Durability The ability of a cement bound material to survive its allotted design life without any signiﬁcant reduction in material quality is an important issue. Surface slabs require a different set of design criteria when compared with cement
- 64. 44 Testing and speciﬁcation bound base materials. Surface abrasion, frost resistance and resistance to chemical attack are issues which are of equal importance in the successful construction of a concrete pavement to the more readily understood structural considerations of tensile and compressive strength. The following key issues are important considerations inﬂuencing the choice of materials. Resistance to abrasion and minimum strength requirement Surface running slabs require a minimum level of strength to avoid erosion from abrasion. The current recommended UK minimum strength (for major highways) is set at a characteristic compressive cube strength at 28-days of 40 MPa. Higher values are suggested in some standards but a 40 MPa mix is the minimum accepted strength threshold to produce abrasion resistance. Surface slab frost resistance and air-entraining Frost damage is a major design consideration for concrete slab systems. A very good summary of the current knowledge on the subject is contained within CIRIA Report CP/69 [14]. A number of different mechanisms which produce frost damage occur; they are described as: • • • surface scaling; production of pop-outs, an aggregate quality problem; d-scaling and various forms of internal structural damage. The basic mechanism of frost damage is generally accepted as a product of the freeze–thaw action of entrapped water within the structure of the concrete matrix. The problem may be prevented by either: • • reducing the size of voids, by adding air entraining agents; Producing a high-strength, dense, voidless concrete; the dense material prevents the formation of ice lenses within the structure of the concrete. The accepted UK and North American method of preventing frost damage is to use air entraining agents. The UK Highways Agency Speciﬁcation [15] uses 5% ± 1.5% air content for 20 mm aggregate. The entrained air prevents damage by allowing the concrete to strain when subjected to the freeze– thaw cycle. An ongoing debate concerns whether very high cement content concrete needs to be air-entrained. Air-entrained concrete has a reduced strength when compared with an equivalent standard mix, but an increased workability, which then allows the water–cement ratio to be lowered, partially compensating for the loss of strength. TRL investigated the effect of air-entraining agents in LR 363 [16]. Table 4.2 presents the strength data recorded within that report.

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment